Engineered Wood Products as a Sustainable Construction Material: A Review

*Ranjana Yadav and Jitendra Kumar*

## **Abstract**

Engineered wood products are considered as best building materials due to environmentally friendly. Huge change to the way in which wood has been utilized in primary application of construction in the course of the most recent 25 years are in light of decreased admittance to high strength timber from growth forests, and the turn of events and creation of various new design of manufactured wood products. Engineered wood products are available in different variety of sizes and measurements like laminated veneer lumber, glued laminated timber, finger jointed lumber, oriental strand board etc. It is utilized for rooftop and floor sheathing, solid structure, beams and the hull of boats. This review objectively explores not only the environmental aspects of the use of different engineered wood composites as a building material, but also their economic aspects, to understand their effect on sustainability.

**Keywords:** engineered wood product, plywood, cross laminated timber, laminated veneer lumber, oriented strand board etc.

## **1. Introduction**

Wood is one of the world's most promptly accessible and adaptable building materials, and recent advances in engineered wood products innovation have permitted these to be utilized in a basically load-bearing segment [1, 2]. Wood has assumed a huge part in the existences of people from ancient occasions to the advanced time. It is richly found in an assortment of normal settings and effectively retrievable in its raw form. Wood has been a fundamental component of development for quite a long time, with saved instances of such constructions dated to millennia B.C. Engineered wood products (EWPs) are among the most excellent and harmless to the ecosystem building materials. In manufacture, they are produced efficiently from a renewable resource. In development, the way that engineered wood products is accessible in wide assortment of sizes and measurements [3].

EWPs are chiefly laminated veneer lumber [4], wood I Beam, glued laminated lumber [5], cross laminated timber [6, 7], finger jointed lumber, oriented strand lumber, oriented stranded board [8, 9], medium density fiber board (MDF) and Particle Board (PB). These EWPs are regularly created from the adhesive bonding of wood chips, pieces or veneers, as well as the mechanical securing of timber segments to frame bigger segments, beams, boards or other structural components [10–14].

The advantages of EWPs incorporate upgraded dimensional stability, the development of bigger and more complex structural segments, decreased impact of common imperfections (for example knots), more noteworthy toughness and more homogenous mechanical properties [15, 16]. These properties of wood can be improved through controlled changes, and this is the establishment of designed wood items [17–20]. This builds the overall performance of structural wood composites, prompting a more viable structure material, accordingly growing potential end uses [21–23]. Engineered wood products have permitted wood to be utilized in circumstances where solid timber is incapable, prompting specific items to help a more different exhibit of uses. This has extended market openings prompting the positive financial development of this industry [24].

As well as being utilized as a substitute for more "traditional" engineering materials, engineered wood products have demonstrated to beat conventional sawn lumber in the structural applications for which they are intended for [25, 26]. Extra advantages of working with engineered wood products include: lower building costs with less expensive materials/speedier construction time, lower ozone depleting substance outflows by not utilizing energy escalated materials, unrivaled adaptability under seismic burdens and better energy execution/effectiveness [27].

As per estimates of Forest survey of India (2017), while the annual production from the natural forests is quite low, the production from the tree outside forest is much higher. Most of the Industrial wood in India is produced from outside government forests and agroforestry/ farm forestry in the country. India is one of the emerging markets in Asia pacific engineered wood industry, currently accounting for 10% of the Asia pacific engineered wood market share. Cross laminated timber market is rising construction industry. Laminated veneer lumber is one of the most popular EWPs.

Engineered wood products are making it conceivable to build taller and bigger wood structures, and there is innovative work on this theme. Hence, this review chapter focusses on various engineered wood products, which are more economical. This review chapter of the current writing offers bits of knowledge. This chapter takes a gander at another age of wood products, made from the sustainable structural material. These products can assume an undeniably significant part in a naturally concerned world.

## **2. Types of engineered wood product**

#### **2.1 Glued-laminated lumber (glulam)**

Glued laminated lumber, or Glulam, is the most essential and oldest member of the engineered wood products family, which has helped with growing the structural uses of wood and conventional sawn wood development [28, 29]. Solid sawn substantial timber is in restricted accessibly for extremely huge sizes, and is not basically proficient because of deformities like bunches and checking. Glulam has disposed of the limitations of utilization of huge sawn wood concerning size of the stem crossarea, the length of the stem, and the structural deformities present. Production of this product started in Europe at when the new century rolled over, in the U.S. in the 1940's, and in Canada in 1952. Glulam individuals comprise of various wood overlays (or "lams") that are fortified together using glue [30–34]. The boards are pressed with hydraulic equipment in the process to ensure tight bonds. Dimensional softwood lumber is regularly picked for the lamination, and care is taken to guarantee that the grain of the boards runs parallel to the longitudinal axis of glulam member (**Figure 1**). Boards utilized in the lamination process may differ in sizes but do not exceed two inches in thickness. Notwithstanding the benefits related with huge

*Engineered Wood Products as a Sustainable Construction Material: A Review DOI: http://dx.doi.org/10.5772/intechopen.99597*

cross-sectional zones, lamination boards are regularly joined at the ends to develop glulam individuals that increased the lengths of stock lumber. Recently, fiber-reinforced polymers have been included in the manufacture of some glulam production [36]. This component enhances the tensile performance of the member and is said to offer economic benefit in some applications [37–42]. Glulam is often used as straight beams, including lintels, purlins, ridge beams and floor beams, Columns including round, square and complex section, curved beams and roofs.

## **2.2 Cross laminated timber (CLT)**

The construction industry is starting to use new enormous scope engineered wood composites known as mass lumber items. CLT is a moderately new wood product that holds extraordinary potential for significantly expanding the utilization of wood products in construction [43–45]. CLT as enormous boards built through the overlay of various layers of structural grade softwood boards. Each layer of boards is usually oriented perpendicular to adjacent layers and glued on the wide faces of each board, usually in a symmetric way so that the outer layers have the same orientation (**Figure 2**). The products are discovering use in building projects as floor slabs, load bearing wall and shear wall [47–49].

**Figure 2.** *Cross-laminated timber [46].*

Being a suitable choice for heavy frameworks manufacturer expanding interest in CLT and giving a green choice to steel and cement. CLT offers high strength and the structural simplicity needed for cost effective buildings, as well as a lighter environmental footprint than concrete or steel. CLT board manufacture considers a wide scope of board sizes and thicknesses. Architect use CLT boards as burden bearing plate components in construction projects, working as floor slabs, rooftops and walls. The substantial idea of CLT and its great strength properties give the likelihood to use in multistory structure. CLT can also be processed as a "readymade" building material, tailoring its process to the precise required measurement to reduce wastage of building material.

## **2.3 Laminated veneer lumber (LVL)**

While glulam and CLT boards are contained wooden boards, various engineered wood products are made with wood veneer. LVL is perhaps the most generally utilized engineered wood products for constructional applications. It is a composite board made from various thin layers of veneers that are lined up with the length of the finished lumber [50–53]. The product was invented in the last part of the 1960's and has gotten grounded as a high strength pillar and header segment in both residential con commercial constructions. Since it is made from veneers, LVL makes up to 35% more powerful utilization of logs than is conceivable with solid lumber. At fabricate, veneers are dried to 8% moisture content, and reviewed for uniform strength and width before lay-up. Adhesive is applied and the board is pressed under heat and consistent pressure until cure (**Figure 3**). Laminated veneer lumber is planned for use as high strength, load carrying beams to help the heaviness of development over window and entryway, and in floor and rooftop frameworks of residential and light commercial wood frame development. It can give the both boards and beam/column components [55].

## **2.4 Laminated strand lumber (LSL)**

LSL is usually realized Timber strand. As of now, LSL is being made from excess, over develop aspen trees that normally are not huge, solid, or sufficiently straight to develop conventionally wood products. In this cycle, the debarked logs are utilized to give the material to chipped strands, which can be up to 300 mm long. These strands are then dried, coated with adhesive, and pressed into huge billets by a process which incorporates steam injection (**Figure 4**). The billet might be up to 140 mm thick, 2.4 m wide and 10metres long. Subsequent to sanding, countless sizes are sliced to suit applications like headers, edge joists for floor frameworks,

**Figure 3.** *Laminated veneer lumber [54].*

*Engineered Wood Products as a Sustainable Construction Material: A Review DOI: http://dx.doi.org/10.5772/intechopen.99597*

**Figure 4.** *Laminated Strand lumber [56].*

columns, joists and studs. It is utilized for a wide scope of millwork, like doors, windows, and practically any item that require high grade lumber. It is additionally utilized for truck decks, fabricated housing, and some structural lumber such as window and door headers [57, 58].

## **2.5 Parallel strand lumber (PSL)**

PSL, ordinarily known Parallam, is intended to supplant huge dimension lumber (beams, planks, and posts). Parallel strand lumber was developed in Canada, advanced onto the market in the last part of the 1980's [59]. PSL comes in numerous thicknesses and widths and is fabricated up to 66 feet in length (**Figure 5**). The strands are for the most part taken from veneers peeled from the outermost part of the logs, where more grain is found. Veneers e are dried to 11% moisture content and reviewed for strength prior to chopping into strands [61]. They are then adjusted parallel to each other, coated with waterproof glue, then pressed and cured [62, 63]. It is utilized for enormous individuals in residential construction and as middle and huge individuals in commercial building construction.

**Figure 5.** *Parallel Strand lumber [60].*

## **2.6 Structural plywood**

One of the most important well-known building materials constructed with veneer is plywood. It is handily sourced from everywhere the world and has exhibited fruitful. Plywood is utilized for some light duty building materials. It is likewise utilized for rooftop and floor sheathing, concrete formwork, webs of wood beams, and surprisingly the frames of boats. It very well may be utilized to oppose gravity loads or to oppose horizontal burdens as in plywood diaphragms and shear walls. Plywood is fabricated from stacked veneers which are organized in an odd number of layers, the grain of the face layers arranged to the long dimension of the board (**Figure 6**). The cross-overlaid lay-up of the veneers gives strength, stiffness and dimensional strength [65].

## **2.7 Oriented strand board (OSB)**

OSB was first produced in Canada in 1964. Since the mid-1980s, OSB has been one of the most commonly used engineered wood-based panels for structural construction in residential sectors due to excellent properties, especially due to the increasingly competitive price [64, 66]. OSB is an engineered structural panel made from strands of wood sliced from small diameter timber logs and bonded together with an exterior grade adhesive, under heat and pressure [67–70]. OSB is manufactured in various grades with improving resistance to the effects of moisture (**Figure 7**). OSB is extensively used for wall sheathing, floor underlayment, roof cover and I-joist in both commercial and residential building. OSB also is used in furniture, reels, trailer liners and recreational vehicle floors [72–74].

## **2.8 Wood I beam**

Wood I beam are engineered wood products which have great strength in respect to its size and weight. Wood I beam is a light beam support assembled by gluing together wooden flanges and fiber board and plywood beams. The flanges of beam made of laminated veneer lumber or finger jointed solid wood lumber. The web of beam made of plywood, laminated veneer lumber or oriented strand board. Wood I beam are available up to 80 feet long (**Figure 8**). It has been used in residential and commercial construction as floor, rood structure of structure and external wall frames. I beam are best for the structure which required rigidity, heat insulation and

**Figure 6.** *Structural plywood [64].*

*Engineered Wood Products as a Sustainable Construction Material: A Review DOI: http://dx.doi.org/10.5772/intechopen.99597*

**Figure 7.** *Oriented Strand board [71].*

**Figure 8.** *Wood I beam [75].*

economy. Nowadays, wood based I beams are becoming popular. Beams allow easy execution of installation penetration. Their 'I' configuration provides high strength and stiffness.

## **3. Advantages of engineered wood products (EWPs)**

The term engineered wood products covers a wide cluster of wood-based items produced using veneers or strands peeled, chipped or sliced. These items are appropriate for construction reason as structural materials [76]. EWPs tend to perform better as they have higher load-carrying abilities compared to solid wood of the same dimension. This is because EWPs have more uniform and predictable structural properties, as the usual deficiencies in the wood (like knots and cracks) are either removed or offset by the manufacturing process. The low cost of engineered wood is the most immediate benefits and the reason that it is so widely used.

The utilization of glue laminated timber offers various benefits including structural opportunity, proficient utilization of timberland asset like the utilization of merchantable and non-merchantable wood species and mixed species application. CLT gives various ecological advantages notwithstanding its excellent thermal performance. CLT boards are produced for explicit end use applications, which bring about almost no waste. (CLT's thick cross segment gives significant imperviousness to fire since boards char gradually [77]. Probably the greatest advantage of utilizing CLT is that the design can be fabricated rapidly and productively. The size of LVL is not restricted by log size, because of its assembling strategy [78]. Since, it is fabricated with homogenous quality that has least number of defects. The advantage of I-joists/beam is they are less likely to bow, crown, twist, up or split as would a dimensional piece of lumber.

Engineered wood product lie plywood permits developers to diminish the quantity of trees required for building a home. Plywood sheathing for walls and rooftops definitely diminishes home construction cost compared with utilizing boards of solid wood. Some engineered products, for example, MDF and PB can be produced using sawmill scraps, wood chips and even saw dust reutilizing wood waste.

Engineered wood product is likewise useful in that it assists with cultivating up the interaction of development. Perhaps the most appealing highlights of these engineered components and assemblies are that they can be manufactured to longer lengths than their sawn lumber partners. Additionally, engineered products preserve or extend the use of the forest resource by using a higher percentage of fiber, which previously was burned or left to rot. The use of wood from residual sources, plantations and second-growth forests reduces the pressure to harvest more forest area. Waste timber can be recycled and turned into strands and fibers and reconstituted into engineered wood products.

#### **3.1 Comparing material options**

In considering the utilization of engineered wood products for a construction, the manufacturer is given a stable of material choices which permit extensive potential for the declaration of sculptural structure. This opportunity to make a masterpiece, when taken, regularly brings about a wood structure whose elegance and excellence is genuinely a supplement to function. It is significant that the wood industry keeps on advancing the advantages of the unique character and warmth of the uncovered structural products. Engineered wood products can be considered as a reasonable substitute or complement for concrete, steel and brick in large building projects.

Simultaneously, it is similarly imperative to know about the premium related with the stock of regularly elaborate shapes and treatments. These may draw structural components as architectural components in a way that utilizes essentially more material that is needed to help a given burden. To appropriately evaluate the expenses of wood versus steel, one should perceive such contemplations. Really frequently, a wood alternative is saved due to such defective examinations. For instance, a school whose structural framework, in the brain of the designer, will be alright served by a structural steel frame and open web steel joist framework ought not just be assembled that way in light of the fact that a weighty wood post and beams framework is costlier. The Engineered Wood Products explained in this chapter currently permit the wood industry to contend with practically identical items to the steel alternative. Cross laminated lumber is able to replace concrete slabs in the frames of multistory buildings [79]. The weight CLT is about 4 times less than concrete which reduces foundation loads and transportation cost. Glulam is two third the weight of steel and one sixth the weight of concrete. The high strength of laminated timbers enables glulam beams to span large distances without intermediate columns, allowing maximum design flexibility than traditional timber construction.

The different sections of this chapter which describe various EWPs refer to the enhanced utilization of logs due to the use of small sections, in many cases veneers or strands. Engineered wood products bring huge advantages compared to *Engineered Wood Products as a Sustainable Construction Material: A Review DOI: http://dx.doi.org/10.5772/intechopen.99597*

competing products such as steel, concrete and aluminum in terms of embodied energy, and emissions of carbon dioxide and other pollutants during manufacture and extraction.

## **4. Conclusions**

This chapter presents an overview of the EWPs. The advancement of new designs of structural wood products – called EWPs- throughout the most recent 25 years has utilized wood fiber and allowed the wood industry to rival other structure materials in more construction applications. Based on the properties and end uses engineered wood products will see an expanding market share within the wood products manufacturing industry. There are various variables impacting this, for example, the advantages of wood building construction, improved fire execution over dimensional timber products. CLT offers high strength and the structural simplicity needed for cost-effective buildings, as well as a lighter environmental footprint than concrete or steel. Current experience shows that engineered wood products are excellent structural wood building material for future.

## **Conflict of interest**

The authors declare no conflict of interest.

## **Author details**

Ranjana Yadav\* and Jitendra Kumar2

1 Indian Plywood Industries Research and Training Institute, Centre, Mohali, Punjab, India

2 Department of Biosciences, University Institute of Biotechnology, Chandigarh University, Mohali Punjab, India

\*Address all correspondence to: ranjanay7@gmail.com

© 2021 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

## **References**

[1] Maxim P, Darryl P, Len G, Joseph C. Taller Wood Buildings and Fire Safety. University of the Fraser Valley; 2013.

[2] Smulski S. (Ed) Engineered wood products. PFS Research Foundation: Madison, Wisconsin; 1997.

[3] Milner HR. Sustainability of engineered wood products in construction. Sustainability of construction materials. wood head publishing series in civil and structural engineering, Cambridge UK; 2009. p. 184-212.

[4] Kurt R, Hayrettin M, Aslan K, Cil M. Laminated Veneer Lumber (LVL) Manufacturing Using Three Hybrid Poplar Clones. Turkish Journal of Agriculture and Forestry. 2012; 36 (2): 237-245.

[5] Moody RC, Hernandez R. Glued-Laminated Timber. In: Engineered wood Products: A guide for specifiers, Designers and Users, Smulski S. (Ed.) PFS Research Foundation, Wisconsin; 1997. p. 1-39. ISBN:096567360X.

[6] Gagnon S, Pirvu C. (eds.) CLT handbook: Cross-laminated timber. FP Innovations, Quebec, Canada; 2011.

[7] Divekar N. Introduction to New material- cross laminated timber. International Journal of Engineering research. 2016; 5 (3): 675-679.

[8] Lowood J. Oriented strand board and waferboard. In: Smulski S (ed) Engineered wood products. Miller Freeman, Madison; 1997. p. 5.123-5.145.

[9] William G. Davids, Habib J. Daugher, Eric D. Cassidy, Douglas G. FRPreinforced oriented strand board panels for disaster-resistant construction, 2003.

[10] Hemmila V, Adamopoulos S, Karlsson O, Kumar A. Development of sustainable bio-adhesives for engineered wood panels–A Review. RSC Advances. 2017; 7 (61): 38604-38630.

[11] Baldwin R. Plywood and Veneers Based Products, Manufacturing Practices, Miller Freeman: San Francisco, California; 1995.

[12] Barbu MC, Reh R, Irle M. Woodbased composites. In Research Development in Wood Engineering Technology, IGI Global. 2014. p. 1-45.

[13] Nelson SPE. Structural composite lumber. In: Engineered wood products a guide for specifiers, designers and users, Sumulski S. (ed.), PFS, Research Foundation, Madison; 1997.p. 147-172.

[14] Shukla SR, Rao RV, Sharma SN. Evaluation of parallel strand lumber (PSL) and 144 WOOD RESEARCH its comparison with laminated veneer lumber (LVL), rubber wood and teak. Holz als Rohund Werkstoff. 1999; 57(4): 267-270.

[15] Lam F, Prion HG. Engineered wood products for structural. Timber Engineering, Wiley, New York; 2003.p. 81.

[16] Nicole MS, Cai Z, Carll C. Wood-Based Composite Materials Panel Products, Glued-Laminated Timber, Structural Composite Lumber, and Wood–Nonwood Composite Materials, Chapter 11, General Technical Report FPL–GTR–190; 2010. p. 11.1-11.28

[17] *Gaff* M, Ruman D, Gašparík M, Štícha V, Boška P. Tensile-Shear Strength of Glued Line of Laminated Veneer Lumber. BioResources. *2016;* 11: 1382-1392.

[18] Gary C W. Engineered wood products - experience and opportunities. NZ Timber Design Journal. 2020; 8 (2):6-13.

*Engineered Wood Products as a Sustainable Construction Material: A Review DOI: http://dx.doi.org/10.5772/intechopen.99597*

[19] Sotayo A, Bradley D, Bather M, Sareh P, Oudjene M, El-Houjeyri I, Harte AM., Mehra S, O'Ceallaigh C, Haller P, Namari S, Makradi A, Belouettar S, Bouhala L, Deneufbourg F, Guan Z. Review of state of the art of dowel laminated timber members and densified wood materials as sustainable engineered wood products for construction and building applications. Developments in the Built Environment. 2020; 1: 100004.

[20] Wang B, Chui YH, He G, Xie D. Development of high performance and durable engineered wood products from mountain pine beetle veneers using novel resin impregnation technologies. Natural Resources Canada; 2009. p. 40.

[21] Smith I, Snow M, Asiz A. Design methods for connections in engineered wood structures, Final Report UNB2, Natural Resources Canada, Ottawa; 2006.

[22] Smith I, Asiz A, Snow M. Performance of mechanical fasteners used with engineered wood products, Final Report UNB75, Natural Resources Canada, Ottawa; 2007.

[23] Snow M. Fracture development in engineered wood product bolted connections [PhD thesis]. University of New Brunswick: Fredericton; 2006.

[24] William C. A Review of Engineered Wood Products in Canada [An undergraduate thesis]. Lakehead University Thunder Bay: Ontario; 2018.

[25] Fadai A, Winter W, Gruber M. Wood based construction for multistorey buildings. The potential of cement bonded wood composites as structural sandwich panels. World Conference on Timber Engineering (WCTE 2012), 2012 ;1. WCTE 2012 Committee. Aukland.

[26] Stark NM, Cai Z, Carll C. Woodbased composite materials: panel

products, glued-laminated timber, structural composite lumber, and wood-nonwood composite materials. In: Ross R. (Ed.), Wood Handbook - Wood as an Engineering Material. U.S. Department of Agriculture Forest Service, Forest Products Laboratory, Madison, WI; 2010. p. 11.1-11.28.

[27] Adair C. Regional production and market outlook tor structural panels and engineered wood products 2001-2006. APA Economics Report E67 Table 28, APA, Tacoma, WA, 2001. p. 51.

[28] Brandner R, Schickhofer G. Glued laminated timber in bending: new aspects concerning modelling. Wood Science & Technology. 2008; 42(5):401-425

[29] Younquist JA. Wood based composites and panel products. In wood handbook: forest product laboratory. United States, department of agriculture forest service, Madison, Wisconsin; 1999. P. 10.1-10.31-113.

[30] Anshari B, Guan ZW, Kitamori A, Jung K, Komatsu K. Structural behavior of glued laminated timber beams pre-stressed by compressed wood. Construction Building Materials. 2012; 29: 24-32.

[31] Anshari B, Guan ZW, Wang QY. Modelling of Glulam beams pre-stressed by compressed wood. Composite Structures. 2017; 165: 160-170.

[32] Correal JF, Echeverry JS, Ramirez F, Yamin LE. Experimental evaluation of physical and mechanical properties of glued laminated guaduangustifolia Kunth. Construction Building Materials. 2014; 73:105-112.

[33] Herawati E, Massijaya MY, Nugroho N. Performance of Glued-Laminated Beams Made from Small Diameter Fast-Growing Tree Species. Journal of Biological Sciences. 2010; 10: 37-42.

[34] Herawati E. The characteristics of glued-laminated beams made from small diameter fast growing species [MS Thesis]. Postgraduate School, Bogor Agricultural University; 2007.

[35] GLULAM. Versatile engineered wood product delivers strength, beauty and reliability, https://ecohousemart.com

[36] Castro G, Paganini F. Mixed glued laminated timber of poplar and Eucalyptus grandis clones. Holz Als Roh-Und Werkstoff. 2003; 61(4): 291-298.

[37] Nadir Y, Nagarajan P. The behavior of horizontally glued laminated beams using rubber wood. Construction Building Materials. 2014; 55: 398-405.

[38] Ezeagu C, Eromosele A, Okoro H, Chukwujekwy U, Emetomo T. Flexural Strength of solid and glue laminated timber beams. American Journal of Engineering Science & Technology Research. 2015; 3 (1): 1-14.

[39] Nagarajan P. The behavior of horizontally glued laminated beams using rubber wood. Construction Building Materials. 2014; 55: 398-405.

[40] Sreeshna KS. Study on Flexural Behavior of Glued Laminated Timber. International Journal of Innovative Research in Science, Engineering and Technology. 2016; 5 (7): 13373-13381.

[41] Vratuša S, Kuzman MK, Kilar V. Structural particulars of glued laminated beams of variable height. Drewno. Pr. Nauk. Donies. Komunik. 2011;54: 185.

[42] Xiao Y, Yang RZ, Shan B. Production, environmental impact and mechanical properties of glubam. Construction and Building Materials. 2013;44: 765-773.

[43] Lehmann S. Developing a prefabricated low-carbon construction system using cross-laminated timber (CLT) panels for multistorey inner-city infill housing in Australia. Journal of Green Building, 2012; 7(3): 131-150.

[44] Liao Y, Tu D, Zhou J, Zhou H. Feasibility of manufacturing crosslaminated timber using fast-grown small diameter eucalyptus lumbers. Construction Building Materials. 2017; 132: 508-515.

[45] Mohammad M, Gagnon S, Douglas BK, Podesto L. Introduction to Cross Laminated Timber. Wood Design Focus. 2012;22: 2.

[46] Dong Y, Cui X, Yin X, Chen Y, Guo H. Assessment of Energy Saving Potential by Replacing Conventional Materials by Cross Laminated Timber (CLT)—A Case Study of Office Buildings in China. Applied Science. 2019; 9: 858.

[47] Arul Mozhi Bharathi DV, Dhanalakshmi E, Manickam K. Study on cross laminated timber. International Research Journal of Engineering and Technology (IRJET). 2020; 7 (9): 1196-1199.

[48] Brandner R, Flatscher G, Ringhofer A, Schickhofer G, Thiel A. Cross laminated timber (CLT): overview and development. European Journal of Wood and Wood Products. 2016; 74: 331-351.

[49] Frangi A, Fontana M, Hugi E, Jubstl R. Experimental analysis of cross-laminated timber panels in fire. Fire Safety Journal. 2009; 44(8): 1078.

[50] Bal BC. Some technological properties of laminated veneer lumber produced with fast-growing Poplar and Eucalyptus. Maderas. Ciencia y Tecnología. 2016; 18(3): 413-424.

[51] Kunesh RH. Micro = Lam: structural laminated veneer lumber. Forest Product Journal. 1978; 28(7): 41-44.

*Engineered Wood Products as a Sustainable Construction Material: A Review DOI: http://dx.doi.org/10.5772/intechopen.99597*

[52] Stump JP, Smith LA, Gray RL. Laminated veneer lumber made from plantation-grown conifers. Forest Product Journal. 1981;31(4):34-40.

[53] Hesterman ND, Gormon TM. Mechanical properties of laminated veneer lumber made from interior Douglas-fir and lodgepole pine. Forest Product Journal. 1992; 42(11/12): 69-73.

[54] Hakkarainen J. LVL Handbook EUROPE. Federation of the Finnish Woodworking Industries, Snellmaninkatu, Finland 2019.

[55] Neuvonen E, Minna S, Jani H, Micha H, Matthias W. Laminated Veneer Lumber - Wood-Based Panels Technology. Laminated Veneer Lumber - Wood-Based Panels Technology. N.p., n.d. Web; 2013.

[56] Laminated strand Lumber. https://images.app.goo. gl/1GiWYAXXKKmk94919.

[57] Wang Z, Gong M, Chui YH. Mechanical properties of laminated strand lumber and hybrid crosslaminated timber. Construction Building Materials. 2015; 101:622-627.

[58] Weight S, Yadama V. Manufacture of laminated strand veneer (LSV) composite. Part 1: Optimization and characterization of thin strand veneers. Holzforschung. 2008; 62(6):718-724.

[59] Ahmad M, Kamke FA. Properties of parallel strand lumber from Calcutta bamboo (*Dendrocalamus Strictus*). Wood Science and Technology. 2011; 45:63-72.

[60] Andre M Iskandar. Potential Market of Parallel Strand Lumber (PSL) and Laminated Veneer Lumber (LVL) in Indonesia. A Report Submitted in Partial Fulfillment of the Requirements for the Degree of Bachelor of Science in Wood Products Processing in The Faculty of Forestry, 2013.

[61] Yihai L, Le W. Selected properties of parallel strand lumber made from southern pine and yellow poplar. Holzforschung. 2003;57(2): 207-212.

[62] Fan MZ, Xu RX, Yang AH. Study on parallel strand lumber made of waste veneer/bamboo strips. Wood Industry (Beijing). 1995; 9(1): 10-13.

[63] Kurt R, Cavus V. Manufacturing of parallel strand lumber (PSL) from rotary peeled hybrid poplar I-214 veneers with phenol formaldehyde and urea formaldehyde adhesives. Wood research. 2011; 56 (1): 137-144.

[64] Structural Plywood. https://images. app.goo.gl/8T8kocPbFfHevuCy5.

[65] Bekhta P, Hiziroglu S, Shepelyuk O. Properties of plywood manufactured from compressed veneer as building material. Materials and Design. 2009; 30 (2009): 947-953.

[66] Mirski R, Dziurka D, Derkowski A. Properties of oriented strand boards with external layers made of non-strand chips. BioResource. 2016; 11: 8344-8354.

[67] Fiorelli J, Soriano J, Lahr FAR. Roof modular system in wood and particle board (OSB) to rural construction. Scientia Agricola. 2012; 6 (3): 189-193.

[68] Barbuta C, Blanchet P, Cloutier A, Yadama V, Lowell E. OSB as substrate for engineered wood flooring. European Journal of Wood and Wood Products. 2012; 70: 37-43.

[69] Dos Santos RBG, Da Costa DF, Bezerra CMVO, Bezerra JFO. Constructive-process of using plates OSB (oriented strand lumber) in sustainable structural systems in a residential building in the city of Manars-AM. International Journal of Advanced Engineering Research & Science (IJAERS). 2019; 6 (10): 85-91.

[70] Cassidy E. Development and Structural Testing of FRP Reinforced OSB Panels for Disaster Resistant Construction. MS Thesis, Department of Civil and Environmental Engineering, University of Maine, Orono, Maine; 2002.

[71] Oriented strand board, Wikipedia. https://images.app.goo. gl/3KA6wHxsw9MqGg5M8.

[72] Gu H, Wang S, Neimsuwan T, Wang S. Comparison study of thickness swell performance of commercial oriented strandboard flooring products. Forest Product Journal. 2005; 55(12):239-245.

[73] Lunguleasa A, Dumitrascu A, Ciobanu V. Comparative Studies on Two Types of OSB Boards Obtained from Mixed Resinous and Fast-growing Hard Wood. Applied Science. 2020; 10: 6634.

[74] Hiziroglu S. Oriented strand board as a building material. Oklahoma State University; 2006.

[75] Voth C, Yadama V. Sustainable Lightweight Wood-Strand Panels for Building Construction, Proceedings of the International Convention of Society of Wood Science and Technology and United Nations Economic Commission for Europe – Timber Committee, Geneva, Switzerland; 2010.

[76] Abeysuriya N. Effective use of structural timber for sustainable construction. http://www. academia.edu*.*

[77] Yu D, Xue C, Yin X, Chen Y, Guo H. Assessment of Energy Saving Potential by Replacing Conventional Materials by Cross Laminated Timber (CLT)—A Case Study of Office Buildings in China. Applied Science. 2019; 9: 858.

[78] Tellnes LGF, Eide S,

Kristjansdottir TF, Kron M. Assessment of carbon footprint of laminated veneer lumber elements in a six-story housing – comparison to a steel and concrete

solution, Chapter 11 - LCA of Sustainable Materials and Technologies; 2011.

[79] Mallo MFL, Espinoza O. Cross-Laminated Timber Vs. Concrete/Steel: Cost Comparison Using A Case Study. World Conference on Timber Engineering (WCTE 2016), Vienna, Austria; 2016.

## **Chapter 3**

## Veneer-Based Engineered Wood Products in Construction

*Elena Vladimirova and Meng Gong*

## **Abstract**

Veneer-based engineered wood products (EWPs) are widely used in construction. Veneer-based EWPs are made of thin veneer sheets or veneer strands with adhesives, mainly including plywood, laminated veneer lumber (LVL), and parallel strand lumber (PSL). This chapter first discusses veneer-based EWPs in terms of their manufacturing, properties, and applications. Secondly, it introduces how veneer sheets or veneer strands intersect with each other in these products, providing additional strength and stable dimensions. Thirdly, this chapter overviews the effects of element dimensions, basic structure, veneer grade, adhesive type, and processing parameters on the properties of these products. Finally, it illustrates the uses of veneer-based EWPs through examples with a focus on their construction applications.

**Keywords:** veneer-based engineered wood products, plywood, laminated veneer lumber, parallel strand lumber, adhesives, engineering properties, structural uses

## **1. Introduction**

Due to the significant population growth and the rising housing standards, the need to use structural wood products has been increasing [1]. At the same time, the timber industry must come up with solutions for ensuring the preservation of natural resources because of the growing demand for lumber and decreasing availability of large-diameter old-growth trees [2, 3]. Previously sawn from massive logs, structural lumber is now made from reconstituted wood in various shapes and sizes, which is classified as engineered wood products (EWPs). EWPs can maximize the use of wood and utilize small-diameter logs in comparison with conventional lumber [3, 4]. There are several types of EWPs in terms of the elements used, such as veneer-, strand-, fiber- and lumber-based EWPs, among which the veneer-based group is the oldest but still widely used.

The veneer-based EWPs, or called layered wood composites, are made of veneer sheets or veneer strands bonded with an adhesive [2], mainly including plywood, laminated veneer lumber (LVL), and parallel strand lumber (PSL), **Figure 1**. These products are largely made from peeled logs and reconstituted wood, which can then be fabricated into large sheets known as engineered panels [7]. The significant advantage of using veneer, as opposed to sawn lumber, is that it can increase the yield of wood materials from logs, particularly from small-diameter logs [8]. Veneer-based EWPs have a more homogeneous structure and uniform mechanical properties than solid lumber, making them a good candidate for building materials in construction.

**Figure 1.**

*Veneer-based EWPs. Top left – plywood (source: photos obtained from Indiamart [5]) top right – thick plywood. Bottom left – LVL, bottom right – PSL (source: photos obtained from think wood [6]).*

Veneer-based EWPs differ by wood species, adhesive type, as well as by layup structure. **Figure 2** shows the cross-sections (i.e., the width-thickness plane, or x-y plane named here) of four widely used wood products in construction, i.e., solid wood/lumber, plywood, LVL, and PSL. In the y-axis, the dimensional change is similar between solid wood, plywood, and LVL due to limited efficacy of adhesive bonds in this direction, i.e., the radial direction of the wood. However, the dimensional change of PSL in the y-axis is smaller than that of the other three products because of its irregular arrangement of veneer strands in the x-y plane and application of an adhesive. On the x-axis, the dimensional change is largest in solid wood (Note: the x-axis is the tangential direction of the wood.) and smallest in plywood

**Figure 2.** *Cross-sections of solid wood and veneer-based EWPs.*

*Veneer-Based Engineered Wood Products in Construction DOI: http://dx.doi.org/10.5772/intechopen.102034*

and PSL, with LVL being in between. In other words, solid wood has the largest variability in both x- and y-axes; plywood and LVL have the reduced variability in x-axes, and PSL has the smallest variability in both x- and y-axis.

The first type of veneer-based EWPs invented is plywood [9]. Later, modifications applied to the veneer layups resulted in LVL, and afterward, the long veneer strands were used to make PSL. The veneer-based EWPs have been widely used in construction nowadays [8]. Plywood is usually used as the sheathing material for walls, floors, and roofs, and the web stock for I-joists. LVL is commonly used as beams, columns, and the flange stock of I-joists. PSL is mainly used as columns and beams.

## **2. Plywood**

#### **2.1 Introduction**

Plywood is a glued wood panel consisting of several thin layers of veneer with wood fibers in adjacent layers at right angles in most cases. Usually, a plywood sheet consists of an odd number of veneer layers [2, 3, 10]. Each layer is called ply, so the plywood can be deemed as a wood sandwich [7]. The cross lamination of adjacent plies in plywood contributes to improved mechanical properties and dimensional stability in both length and width directions [10].

Plywood is one of the oldest veneer-based EWPs. More than 3500 years ago, a type of plywood was found in ancient Egypt, which is part of the coffin, dating back to the third Egyptian dynasty [8]. Later, around 1500 BC, some images were discovered in which workers cut plywood with an axe-like tool. These images also show that the glue, apparently of animal origin, was prepared in a pot on fire [6]. Furniture constructed from overlapping sheets of wood and inlay had been discovered in Egyptian tombs. Hardwood veneer was preferred due to its attractive texture and shades [11]. The introduction of plywood was linked to the high cost of wood. Due to the shortage of available wood than supply, Egyptians had to import, by sea, ebony and mahogany from East Africa and cedar and pine from Lebanon at a very high price [12]. Later, the ancient Greeks and Romans started producing plywood. Plywood was primarily used for the manufacturing of furniture and household items [11]. Plywood production took off in the 1850s thanks to the Swedish inventor Emmanuel Nobel, who created a model of a rotary lathe [8]. This model made it possible to remove the veneer in a certain and constant thickness from a wooden block. It gave the plywood a uniform thickness and structure [8].

Despite the fact that plywood is now widely used for sheathing in residential and commercial construction, early builders were hesitant to use the newly-born plywood panels because the blood and soybean protein-based glues used were not waterproof, and some panels delaminated when they got wet [13]. In 1934, waterproof synthetic wood adhesives were introduced, which solved the problem and eased builders' concerns [8, 13]. During World War II, the use of plywood was exploded in many industries such as boats, aircrafts, footlockers, crates, and buildings [13]. It led to the post-war boom in plywood production [8], which was adopted for structural and exterior applications. One notable example of using plywood is the construction of the legendary bomber Mosquito [14]. This aircraft was introduced during the World War II. Spruce wood, birch plywood, and balsa wood were used in the construction of aircraft, which made it possible to achieve the necessary strength with a low weight structure [15]. Plywood and other structural panels have changed the way of constructing light wood-frame houses and buildings [11, 16]. Since the middle of the past century, usage of structural panels has

expanded from a few niche applications to a popular commodity such as subflooring, roof and wall sheathing, corner bracing, and concrete forming [16]. Initially concentrated in the Pacific Northwest of the United States, where old-growth, large-diameter Douglas-fir was mostly used the plywood business therefrom expanded into the southeastern regions in the 1970s as the technological barrier of bonding southern yellow pine veneer was removed [13]. As seen from **Figure 3**, plywood consumption in Canada was rather stable in the last 15 years or so despite the emergence of other new types of building materials. However, Canada also imports plywood from other countries to meet its increasing demand in construction and other industries such as furniture [17].

### **2.2 Manufacturing**

**Figure 4** illustrates the key processes of manufacturing three major veneerbased EWPs, i.e., plywood, LVL, and PSL. An example of manufacturing Canadian softwood plywood is given below, which is used for structural applications. Specially chosen peeler logs are transported to a barker, where they are rotated against a steel claw, which removes the bark [18]. Then debarked logs are cut into peeler blocks. A block is placed on a massive lathe, rotating against a sharp knife. When the block turns, a continuous thin layer of wood, i.e., veneer is peeled off, similar to how paper unwinds from a roll.

The whole block is tried to use with an aim to generate a high yield of good quality wood material. The leftover small spindles are used to make other wood products. The long ribbon of the veneer is then cut with clippers into desired widths and sorted. It is also possible to remove defective pieces of veneer. Subsequentially, the veneer is dried to a moisture content of 5% or so in steam- or gas-heated ovens [18]. Depending on its intended use, the veneer may range in thickness from 0.3 mm (0.01 in) to 6.3 mm (0.25 in) [11]. After drying and sorting, the veneer is fed by glue spreaders, which apply an adhesive layer of uniform thickness. Phenol-formaldehyde (PF) adhesives are usually used in the manufacturing of plywood for structural and outdoor applications when exposed to the weather in its service [3]. Veneer sandwiches are sent to the hot press, which is a key step in the production process of curing the adhesive, subjected to a temperature of 150°C (300°F), and a pressure of 1.38 MPa (200 psi). After the press panels are cut to required dimensions, sanded, and graded [18].

In the fabrication of plywood for non-structural uses, such as furniture, cabinets, and indoor decoration, water-resistant urea-formaldehyde (UF) adhesives are used. The UF adhesives can be cured at a temperature of about 120°C (250°F) during hotpressing, which can also be cured with high-frequency heating system with an aim to reduce the hot-pressing time and increase the production efficiency [3].

**Figure 3.** *Plywood production and consumption in Canada [17].*

*Veneer-Based Engineered Wood Products in Construction DOI: http://dx.doi.org/10.5772/intechopen.102034*

**Figure 4.** *Processes of manufacturing veneer-based EWPs.*

Quality control, which includes incoming management of raw materials, such as wood and glue, and manufacturing parameters at all stages of the production, must be applied in order to produce good quality plywood products. Acceptance quality control is the final stage of the manufacturing process. Many plywood manufacturers in western Canada produce structural plywood under the supervision of the British Columbia Council of Forest Industries (COFI), which constantly checks glue bond strength and other properties to guarantee that the products satisfy the Canadian Standards Association (CSA) standard [18].

## **2.3 Typical species and sizes**

Plywood can be made from various types of wood. Softwoods are commonly used to make veneer for plywood in North America, containing Douglas fir, western hemlock, spruces, pines, and firs [14]. These wood species can be divided

into various categories based on their strength and use within the plywood structure. Spruce is used to make the majority of construction-grade softwood plywood in Canada [7]. More discussion on softwood plywood is given through the text in following sections.

Of hardwoods, birch, alder, linden, and lauan ("Philippine mahogany") are most popular for veneer production [7, 10]. These species do not have distinguished earlywood and latewood zones, which are characterized by uniform density and structure, making them easy to be peeled to produce thin and durable veneer.Beautifully grained hardwoods are often combined in several ways to make a unique face pattern [7].

The first standard plywood sheet had a width of 1.22 m (4 ft) and a length of 2.44 m (8 ft), which appeared in 1928 [19]. Such a standard size for plywood sheets has, since then, almost not been changed. The common thickness of plywood varies from 3.2 mm (1/8 in) to 76 mm (3 in) [10]. It depends on the thickness of the veneer and the number of layers. The most common plywood contains 3, 5, or multiple layers. With a three-layer, the plywood is 2–3 mm (0.08–0.12 in) in thickness, which can be used as an underlayment between the subfloor and the tile. Hardwood decorative plywood is often uniformly selected for grain texture, which is widely employed for indoor uses. The universal hardwood plywood has five layers, resulting in a thickness of 4 mm (0.16 in) or so, which can be used for multiple outdoor and indoor applications. Multiple layer plywood with more than seven layers can be classified as thick plywood, which is widely used for structural purposes, requiring acceptable strength and durability under the loading condition [11]. The thick plywood needs a sub-floor or structural sheathing attached to the framing elements of a new canopy.

Hardwood can be peeled or sliced for the production of decorative veneer for making furniture, cabinets, and interior decoration. Slicing results in more loss in raw materials and more intensiveness in labor [16]. Hardwood veneer, such as birch, usually has a thickness of 1.5 mm (0.06 in), whereas softwood veneer is often cut to a thickness of 3 mm (0.12 in) for plywood and LVL production [8].

#### **2.4 Grading**

Plywood comes in a range of appearance grades, from flat natural surfaces suitable for finishing to cost-effective unsanded grades suitable for sheathing. More than a dozen typical thicknesses and over twenty different grades of plywood are available [14]. The plywood is usually graded based on the appearance quality of veneer in North America. There are commonly two classes of plywood, each of which has its own set of standards: (a) construction and industrial plywood and (b) hardwood and decorative plywood [3].

In Canada, the two most popular types of softwood plywoods are unsanded sheathing grade Douglas Fir Plywood (DFP), which conforms to CSA O121 "Douglas fir plywood", and Canadian softwood plywood (CSP), which conforms to CSA O151 "Canadian softwood plywood". The poplar plywood, which conforms to CSA O153 "Poplar plywood", is also designated but less uses in construction [14]. The group of DFP can include other species in addition to Douglas fir. For example, the front and back faces are made of Douglas fir, but the inner plies can be made from any of the specified species, including Douglas fir, western hemlock, and the majority of spruce, pine, and fir species in Canada [14]. Plywood that contains other selected Canadian wood species in the face and back plies is labeled CSP. Most species that are only allowed as inner plies for DFP may also be used as the face or back plies for CSP. Three hardwood species, i.e., balsam poplar, trembling aspen, and cottonwood, are restricted to use as inner plies in DFP and CSP [14]. The sizes, grades, specialty panels, manufacturing tolerances, and glue bond quality of plywood are all stipulated in the standards CSA O121, CSA O151, and CSA O153.

The structural plywood is put with a legible and durable stamp showing the manufacturer, the bond style (EXTERIOR), the species (DFP or CSP), and the grade [14]. DFP and CSP are both made in a variety of grades based on the appearance and quality of the veneer used for making the outer plies.

Many plywood mills are members of the associations, which are responsible for inspecting, testing, and certifying the products with stamps. These stamps indicate that the stamped products meet the standards accepted by the associations. One of the largest associations in North America is APA – The Engineered Wood Association (formerly American Plywood Association) [20]. There are usually two letters on a stamp, the first indicating the quality of one surface, while the second showing the quality of the opposite surface, **Figure 5** [7]. This stamp ensures the customer that this product has followed the association's stringent quality and efficiency standards [3]. In Canada, the CertiWood™ Technical Center (formerly CANPLY– the Canadian Plywood Association), a non-profit, industry-funded association, represents manufacturers of EWPs [21]. Those mills, being the members of CertiWood™ Technical Center, can put the stamp with the trademark CANPLY on their products [7, 21].

The vast majority of construction and industrial plywood is used in applications where structural performance surpasses appearance. Some construction and industrial plywood are manufactured with faces chosen mainly for appearance of either plain natural finishes or lightly pigmented finishes [3]. Structural plywood is available in two exposure durability classes: interior and exterior [13]. INTERIOR plywood is only intended for use in dry indoor applications where the panels should be protected from moisture permanently; which is even glued with a water-resistant interior-use adhesive [13]. EXTERIOR plywood is the only panels suitable for outdoor exposure. They are bonded with a waterproof exterior-use adhesive [13], including EXPOSURE 1 and EXPOSURE 2. EXPOSURE 1 panels are waterproof and designed for applications where long construction delays or exposure to high moisture in service are possible [13]. EXPOSURE 2 panels are water-resistant and designed for protected applications, where only minor construction delays are expected since they are mainly developed for interior use [13]. Sheathing grades that are not listed for appearance usually have the grading stamp on one of the faces, whereas grades such as Good Two

#### **Figure 5.**

*A sample stamp on plywood: 1- panel grade - panel grades are generally identified in terms of the veneer grade used on the face and back of a panel (e.g., A-B, B-C); 2- bond classification - exposure ratings for APA wood structural panels may be exterior or exposure 1; 3 - decimal thickness declaration; 4 - mill number manufacturing mill identification number; 5- species group number - classified according to strength and stiffness under manufacturing standard; 6 - product standard [20] (source: photos obtained from APA – the Engineered Wood Association [20]).*

Sides are stamped on the edge to avoid affecting the appearance. The strength values stipulated in CSA O86 "Engineering design in wood" [22] are used for Sheathing grade panels based on layups containing only C-grade veneer. Typical DFP and CSP grades include Sanded grades, primarily used in concrete formwork or non-structural applications, and Select and Select Tight Face grades, which are primarily used in floor underlayment applications requiring a smooth and solid surface [14].

Chemical treatments can be applied to plywood to increase its resistance to decay and fire. In Canada, the preservative-treated plywood must be made following CSA O80 "Wood preservation" [23]. To assess the effects of fire retardants or some other potentially strength-reducing compounds, plywood producers shall conduct tests following ASTM D5516 "Standard test method for evaluating the flexural properties of fire-retardant-treated softwood plywood exposed to elevated temperatures" [24] and ASTM D6305 "Standard practice for calculating bending strength design adjustment factors for fire-retardant-treated plywood roof sheathing" [14].

#### **2.5 Properties**

The density of plywood depends on the wood species and thickness used, which varies from 400 kg/m3 (25 lb./ft3 ) to 800 kg/m3 (50 lb./ft3 ) [3]. This is compared to the density of oven-dry wood, ranging from approximately 320 kg/m3 (20 lb./ft3 ) to 720 kg/m3 (45 lb./ft3 ) [3]. Plywood has good machining properties; thus, it is possible to work with it just like with ordinary wood, such as sawing, nailing, and gluing. However, the cross-lamination design of plywood, in contrast to wood that is broken down the grain, prevents it from splitting readily in the grain direction. As a result, screws and nails can be used in structural applications near the edges of plywood panels.

Plywood has exceptional built-in resistance to raking, twisting, or distortion, which is especially crucial when care is taken for transferring large shear stresses generated by powerful winds or earthquakes [11]. Many strength properties are equalized by changing the direction at 90 degrees to the grain with each consecutive wood layer of veneer. This provides plywood with a two-way capacity, i.e., the properties in the width direction are approximately equal to those in the length direction. For example, 6 mm (1/4 in) sheathing plywood on a typical framed construction wall with doors and windows delivers double the rigidity and strength furnished by 19 mm (3/4 in) thick boards laid diagonally. When glued to the framework, the strength values for plywood walls are raised even further [11].

Because structural plywood uses waterproof resins, a weather-resistant panel can be obtained if the edges are properly sealed [10]. Awareness of the allowable design values of a plywood panel is not required except in special engineering applications such as diaphragms and earthquake-resistant shear walls. When properly fastened to framing at the correct spacing, the span ratings alone ensure that the panels can work well under the roof and floor loadings stipulated in the building code. In North America, the design values can be found in CSA O86 "Engineering design in wood" [22], Wood Design Manual [25], and APA – Plywood Design Specification [20] or in its Design Capacities of APA Performance-rated Structural-Use Panels Technical Note N375 [26]. For engineering applications, STRUCTURAL I panels are typically the best choice. The typical values of sheathing grades are listed in **Table 1.** The properties of plywood vary with the quality of the constituent layers.

#### **2.6 Applications**

Plywood is widely employed in structural and non-structural applications [3], which can be an ideal option for use in both wet and dry environments [14]. It was *Veneer-Based Engineered Wood Products in Construction DOI: http://dx.doi.org/10.5772/intechopen.102034*


**Table 1.**

*Mechanical properties and testing standards of plywood (source: Wood Engineering Handbook [27]).*

reported that plywood took about 54.8% of the market share in 2017 in the construction sector in North America **Figure 6** [21].

In construction, plywood is mainly used as a load-bearing element in platformframe structures, including single-family and multi-family housing, such as sheathing and underlayment, since it has good dimensional stability and does not crack, cup, or twist [18]. Plywood panels are used as wall sheathing materials, providing high lateral resistance to shear walls and high racking strength, and assisting in achieving the overall thermal efficiency of walls [16, 18]. Roof sheathing is frequently made of plywood. The stiffness of which constitutes diaphragm action when using prescribed framing and nailing patterns [18]. Also, plywood often finds its uses in the fabrication of I-joists as web stocks, marine applications, pallets, industrial containers, and furniture, **Figure 7**. Extra thick plywood with special surface treatment can be used for facing concrete formwork in concrete structures [7, 10, 14].

#### **Figure 6.**

*North America plywood market share by segment in 2017 (source: Figure obtained from BCC research, FAO, RAUTE, IMF, National Statistics Offices [33]).*

Plywood webs making I-joists

**Figure 7.** *Plywood applications [20, 34–36].*

## **3. Laminated veneer lumber (LVL)**

## **3.1 Introduction**

Laminated veneer lumber (LVL) is a type of structural composite lumber (SCL) made by gluing several layers of veneer in the longitudinal direction of the wood, which differs from plywood that has the veneer layers cross-laminated. LVL is one of the most important members in the family of veneer-based EWPs [8]. This material was initially used to produce aircraft propellers and other high-strength aircraft components during World War II [18, 37]. The research and development of LVL can be dated back to the 1940s with an aim at making high-strength parts for aircraft structures out of Sitka spruce veneer [3]. LVL was used as a building material since the mid-1970s [18, 37, 38] when the research was focused on examining the effects of manufacturing variables on LVL with a thickness being up to 12.7 mm (1/2 in) [3]. LVL is now widely used as building and packaging materials [18].

## **3.2 Manufacturing**

The veneer manufacturing and drying processes are almost the same as those used in making plywood. **Figure 4** illustrates the different processes in the manufacturing of LVL from plywood, largely including veneer orientation during layup, hot press type, and end cutting to produce the length required.

*Veneer-Based Engineered Wood Products in Construction DOI: http://dx.doi.org/10.5772/intechopen.102034*

To make veneer sheets, the logs are usually peeled in a lathe. The thickness of veneer sheets in 1.5 mm (0.06 in) up to 6.4 mm (0.25 in) [16, 38], the length is 2640 mm (104 in), and the width is 1320 mm (52 in) or 660 mm (26 in) [18]. The veneer is dried to a moisture content of 6–10%, ideally 6–8% [38]. The veneer is clipped to remove any strength-reducing defects and graded. The veneer sheets are cut to the desired width for billet production [18]. The individual veneer sheets are then joined, with the grain of all veneers running in the direction of a billet's length direction. End joints between different veneer pieces are staggered along the length of the billet to distribute any defects that could reduce strength. To effectively transmit load, the joints might be scarf joined or overlapped for some distance [18]. Then the veneer sheets are covered with a waterproof phenol-formaldehyde adhesive [18, 37, 38] or phenol-resorcinol-formaldehyde or polyurethane adhesives [39].

The veneer layup of LVL differs from that of plywood. In the production of LVL, the veneer is oriented in the same direction, i.e., the longitudinal grain direction of the wood, providing the super strength in this direction, which is similar to or larger than solid lumber, **Figure 8**. Thus, LVL is commonly used for beams and columns in the construction of buildings [8, 10]. Veneer sheets in plywood are crosslaminated, making it possess two-way properties, i.e., similar properties in both major and minor directions, as mentioned in Section 2, suitable for sheathing materials.

The pre-pressing of LVL billets could be carried out in a single-opening cold press or a short continuous cold press [38]. The completed billets are simultaneously exposed to pressure to consolidate the veneer and heat to accelerate the curing of the glue [18]. In general, the press temperature used to produce LVL is rarely higher than 175°C (350°F). For the batch type presses, it is usually 160°C (320°F). For the continuous presses, the temperature might be significantly higher since there is a pre-heating zone. As veneer sheets are relatively low in permeability, it is recommended to avoid using a high press temperature, especially when combined with a long press time [38]. This process is similar to used in manufacturing of plywood, except that instead of being formed into thin flat panels, the veneer sheets for making LVL is formed into long billets up to 25 m (80 in) in length. After curing, the billets are sawn to specific lengths and widths for the target application(s) of a LVL product [18].

**Figure 8.** *Layups of LVL and plywood (source: image obtained from Gong [39]).*

During the manufacturing of LVL, the selection of veneer is, in terms of thickness and grade, of great importance. The right veneer thickness can help balance LVL properties and manufacturing costs in the production. The veneer used in the manufacture of LVL must be carefully selected in order to obtain the desired engineering properties. Ultrasonic scanning is often used to sort veneer sheets to ensure that the final product has the desired engineering properties [37]. The individual veneer is typically graded so that the strength characteristics of each LVL can be customized [10]. For esthetic reasons and superior flatwise bending properties, the best veneer sheets are usually used as surface plies, while lower-grade sheets are used for the inner plies [38]. For example, if the final use of LVL is scaffold planks, the higher grade veneer will be put on the plank's outer sides [18].

With decreasing veneer thickness, the number of veneer sheets required increases for the same density, thickness, and layout technique of an LVL product. As a result, defects in LVL with thinner veneer will disperse more defects than in LVL with thicker veneer. Because of this, as the veneer thickness decreases, the variation diminishes, and the strength values increase. However, as veneer thickness decreases, resin content, press cycle time, and production cost increase [38].

The strength properties of veneer are more critical for LVL than those in plywood in general. As a result, it is highly desirable for LVL producers to avoid using the veneer sheets with deep lathe checks that cause a reduction in veneer strength. Deep lathe checks can decrease LVL's shear strength and stiffness while having little effect on its MOE. Low shear rigidity can reduce LVL's MOE rating [38].

#### **3.3 Typical species and sizes**

LVL can be made from different softwood and hardwood species; however, in North America, Douglas-fir, larch, southern yellow pine, hemlock, aspen, and yellow poplar are the most widely used wood species for producing LVL [18, 37, 40].

LVL is available in thicknesses ranging from 19 mm (3/4 in) to 89 mm (3–1/2 in) and likely to 178 mm (7 in) [18, 41]. The most typical thickness of LVL used in construction are 38 mm (1–1/2 in) [3] and 45 mm (1–3/4 in) [18], from which broader beams can be conveniently assembled on a job site by fastening several LVL plies [18]. The typical depth is from 140 mm (5–1/2 in) to 508 mm (20 in). Different manufacturers can also provide different widths and depths. At the job site, LVL can easily be cut to a length required [37]. Typical lengths of LVL are 14.6 m (48 in), 17 m (56 in), 18.3 m (60 in), 20.1 m (66 in), and 24.4 m (80 in) [10, 37, 41]. LVL is manufactured in the form of billets with widths of 610 mm (24 in) or 1220 mm (48 in). The required depth of LVL can be cut from these billets [18].

#### **3.4 Grading**

LVL is a proprietary product; therefore, its engineering properties and sizes can differ from one manufacturer to another. As a result, there is no general production standard or design values in the LVL industry [37]. However, the Canadian Construction Materials Centre (CCMC) reviews and approves the design values, which are derived from test results following CSA O86 "Engineering design in wood" and ASTM D5456 "Standard specification for evaluation of structural composite lumber products" [37]. Each manufacturer develops the characteristic properties of its LVL products by in-grade testing. The manufacturer is also responsible for checking the properties of its products by constant monitoring and quality management. Each manufacturer publishes its own list of design properties, resulting in a unique grade for a given LVL product [42]. Products that satisfy the CCMC criteria are assigned an Evaluation Number and an Evaluation Report that

describes the design strengths. They are then entered into the CCMC's Registry of Product Evaluations. The manufacturer's name or product marking, as well as the stress grade, are stamped on the material at different intervals, although this may not be present on every piece due to end cutting [37].

**Figure 9** presents a stamp of LVL from APA – The Engineered Wood Association, which shows a qualified LVL grade (e.g., 3100Fb-2.0E), product evaluation reports, the treatment facility, and standard specifications for SCL.

## **3.5 Properties**

The density of LVL is about 480–510 kg/m3 (30-32 lb./ft<sup>3</sup> ) [43], which is similar to that of the wood made from. Compared to solid wood, LVL has more stable characteristics than solid timber. This is due to the fact that natural defects, such as knots, splits and slope of grain, are dispersed throughout the material or completely removed during the manufacturing, and dried veneer and adhesives are employed [37].

LVL can easily absorb water, resulting in the change in dimensions, in particular in the thickness direction since there are almost no adhesive restrictions. Therefore, LVL should be protected from the weather during job site storage and after installation [3, 37]. Wrapping the LVL materials for shipping to the job site is also critical for minimizing the moisture effect. End and edge sealing are the commonly used approach to avoid moisture penetration and protect LVL products in their services [37].

Both special cutting, notching, or drilling should be performed according to the manufacturer's instruction. LVL acts similarly to solid sawn timber or gluelaminated beams of equal height, which requires the same fastening and connection requirements as solid lumber [40]. The primary sources of knowledge for design, standard installation descriptions, and performance characteristics are provided in the manufacturer catalogs and inspection reports [37].

#### **3.6 Applications**

LVL is mainly used as structural framing in residential and industrial buildings. In the building industry, LVL is widely used for beams or headers over windows and doors on the edge, for hip and valley rafters, scaffold planking, and the flange material of I-joists [3, 10]. LVL may also be used as truck bed decking and road signposts. LVL is chiefly used as a structural component, most commonly

#### **Figure 9.**

*LVL stamp: 1 – qualified LVL grade (usually represented by design values; 2 – APA mill number; 3 – product evaluation reports; 4 – standard specification for structural composite lumber (source: photo obtained from APA – the Engineered Wood Association).*

#### **Figure 10.**

*Curved LVL structures at Simon Fraser University (Canada) - Ripple Cone Canopy (source: photos obtained from StructureCraft [44]).*

in hidden spaces where esthetics is not a concern. Certain manufacturers offer a finished or architectural grade look, but it typically comes at a cost. When using LVL in applications where esthetics is significant, standard wood finishing techniques may be used to accent the grain and preserve the surface layer. The finished wide outer layer of LVL looks like plywood [37]. **Figure 10** shows such a complex curved structure constructed Burnaby, British Columbia, Canada, which was designed and built with 53 parallel CNC-cut spruce LVL sections [44]. Each curved structure was panelized into six segments, shipped to the construction site, and assembled into one piece [44].

Veneer-based EWPs have also been used in the windmill industry, in which wood veneer sheets are used to make windmill blades [45]. Previously, the size of the wooden blade was constrained by the availability of large, consistent-quality tree trunks. Veneering, on the other hand, spreads out defects like knots, resulting in more substantial and more predictable stiffness properties. This makes it possible to make larger wooden blades. When compared to fiberglass, wood laminates provide substantial cost and reduced weight. There are examples of blades made primarily of LVL reinforced with carbon composite spars and coated with a fiberglass composite outer layer [46]. One of the largest windmill blades is 107 meters long (351 ft), which is longer than a football field, produced in Cherbourg, France. It was made from a high-tech sandwich structure consisting of thin layers of glass and carbon fibers and balsa wood veneer [47].

## **4. Parallel strand lumber (PSL)**

#### **4.1 Introduction**

Parallel strand lumber (PSL) is known as a composite of veneer strands with wood fibers aligned primarily along the length of the member, i.e., the longitudinal direction of wood [3]. PSL is overall similar to laminated strand lumber (LSL) and oriented strand lumber (OSL) but is made up of veneer strands (sometimes called veneer strips). The length of veneer strands used in PSL is longer than the strands used in LSL and OSL, with a length-to-thickness ratio of around 300.

PSL was invented in 1975 by MacMillan Bloedel Ltd., in Vancouver, Canada, who set out to create a high-strength wood-based material [13]. The first PSL plant was opened in 1982, and its products were first commercially sold for Expo '86. MacMillan Bloedel, which is now called Weyerhaeuser, commercialized and patented its PSL products with the brand name Parallam®. The process has been improved over time to produce relatively giant and long beams, and the production and sales have steadily increased [48].

## **4.2 Manufacturing**

The process of manufacturing PSL allows prominent members to be built from small trees, resulting in the more efficient use of forest resources [49]. The first stages in the production of PSL are similar to those used in the production of plywood or LVL. **Figure 4** illustrates the unique processes employed in the manufacturing of PSL, differentiating from those in plywood or LVL. To make veneer, logs are turned on a lathe [18]. The thickness of veneer is from 3 mm (1/8 in) to 6.4 mm (1/4 in) [3]. The veneer sheets are then dried to a moisture content of 2–3% before being sliced into long thin veneer strands parallel to one another [9]. After that, the veneer sheets are clipped into long, narrow veneer strands with a length of 2.4 m (8 feet), a width of 13 mm (1/2 in) [18], and a thickness from 2.54 mm (1/10 in) to 3.175 mm (1/8 in) [38].

The production process is designed to use materials from the log roundup and other less than full-width veneer in the veneer cutting stage. As a result, the process uses waste materials from a plywood or LVL operation [3]. The veneer strands are oriented to the length direction of a continuous billet using special equipment (**Figure 11**) and mixed with a waterproof exterior structural adhesive, such as phenol-formaldehyde, prior to hot-pressing.

The pressing process densifies the veneer strands to some degree, and the adhesive is cured with the aid of microwave technology [18, 49]. A continuous press is employed to produce PSL, which theoretically produces an unlimited length but is constrained only by transportation restrictions [3].

## **4.3 Typical species and sizes**

Douglas fir is used to produce PSL in Canada, and southern yellow pines are employed in the USA. In addition to this, western hemlock and yellow poplar are also used [3, 49, 51]. In general, there are no restrictions on the use of other wood species.

The available stock sizes for PSL have to be compatible with existing wood framing materials and standard dimensions [18]. PSL beams are available in thicknesses

**Figure 11.** *Orientation of veneer strands in PSL (source: photos obtained from WorldPress.com [50]).*

from 89 mm (3–1/2 in) to 178 mm (7 in), and in-depth from 235 mm (9–1/4 in) to 457 mm (18 in) [41]. PSL columns come in square and rectangular shapes of a dimension of 89 mm (3–1/2 in), 133 mm (5–1/4 in), or 178 mm (7 in) [41]. Smaller thicknesses can also be used, either individually as single plies or in combination for multi-ply applications [18, 49]. Steel connectors are usually required for larger dimensions [51]. PSL is available in lengths up to 20 meters (66 ft) [41].

The beam-like PSL products can be also ripped into thin boards, **Figure 12**, which opens a window for non-structural applications [18].

### **4.4 Grading**

PSL is a proprietary product, the same as LVL. Therefore, specifications and dimensions are unique to each manufacturer. In North America, both PSL and LVL are treated as the same structural composite lumber [18]. The evaluation procedure and grade determination of PSL are the same as LVL (refer to Section 3.4). **Figure 13** presents a stamp of PSL (Parallam® Plus), including a description of the product and uses, the type of treatment, and the treatment facility. The treatment stamp can also reference the treating standards (such as AWPA U1/UC4A by the American Wood Protection Association) and third-party quality program monitor (SPIB - Southern Pine Inspection Bureau) [53].

#### **4.5 Properties**

Since natural defects such as knots, the slope of grain, and splits have been scattered across the material or eliminated during the manufacturing process. The combination of a structural adhesive used with dried wood veneer strands, heat, and pressure employed during pressing makes PSL less warping than solid timber. Therefore, PSL is a type of highly consistent, uniform EWPs [49], which exhibits much less variability and larger load-bearing capabilities than solid lumber [51]. The density of PSL is 720 kg/m3 (45 lb./ft<sup>3</sup> ) [54], which is similar to that of the wood used. Other advantages of PSL are given to its high strength, stiffness, and dimensional flexibility [49]. PSL is less susceptible to shrinkage, warping, and splitting as it has a moisture content of 11% [49].

The texture of PSL is rich due to the grain of wood veneer strands and dark glue lines. PSL is a visually appealing construction material that fits well to the applications that require a high level of finished appearance [49]. The techniques applicable to sawn lumber can be used to machine, stain, and finish PSL. At the end of the manufacturing period, PSL is sanded to ensure exact dimensions and a high-quality appearance. Stain can be used to emphasize the warmth and texture of the wood [49]. It should be pointed out that the special cutting, notching, or drilling of PSL shall be performed in compliance with the manufacturer's instruction.

**Figure 12.** *Boards ripped from PSL (source: photos adopted from Goulddesigninc.com [52]).*

#### **Figure 13.**

*Stamp on PSL (Parallam® plus) (source: image obtained from Weyerhaeuser [53]).*


#### **Table 2.**

*Major strength properties of SCL (source: Canadian Wood Council [41]).*

As mentioned above, both PSL and LVL are treated as the same SCL in Canadian practices; therefore, their design values are the same. **Table 2** lists the key strength properties of sample SCL. Some specific design values can be obtained from manufacturers [41].

## **4.6 Applications**

PSL is mainly used in residential, commercial, and industrial construction as structural framing components, such as beams and columns in the postand-beam construction, and headers, pillars, and lintels in the light-frame construction [18]. According to Part 3 of the National Building Code of Canada, CCMC has approved PSL for use as heavy timber construction [51]. Due to the excellent strength characteristics of PSL, it is possible to use it in the design of the roofs with a large span and rooms with open spaces. **Figure 14**(left) presents PSL beams that are used for an open floor plan at Vancouver Firehall No.15, Vancouver, Canada. Another example is presented in **Figure 14**(right), showing a portable Concord Pacific Display Pavilion at Vancouver, Canada, which uses a glass-enclosed superstructure made of exposed PSL columns. In addition, PSL is a visually attractive material; thus, it is well suited to applications where the finished look is essential. It can be also appropriate for hidden structural applications where appearance is unimportant [18].

#### **Figure 14.**

*Floor and columns made of PSL in Vancouver Firehall No.15 (left) and Concord Pacific display pavilion (right), respectively (source: photos obtained from StructureCraft [55]).*

## **5. Endnotes**

EWPs are relatively recent structural members that have been widely incorporated in the building industry in North America and beyond. They have been invented and used for making timber buildings and furniture. The family of veneerbased EWPs mainly has three major members, i.e., plywood, LVL, and PSL. Because the majority of veneer-based EWPs are designed to handle relatively large loads, they must be manufactured in accordance with recognized standards or technical guides to ensure that the required engineering design values and applications are met. Veneer-based EWPs have been accepted and acknowledged in the building industry as premium structural materials. It is possible to make these products considerably large from small-diameter logs. The only restriction can be the length of LVL and PSL during transportation [38].

Non-traditional resources (such as under-utilized wood species) can be used to manufacture veneer-based EWPs of better physical and mechanical properties than other traditional structural products (such as solid timber products) [1]. Due to engineering design, removal of defects, drying of wood materials, application of adhesive, and layer-by-layer bonding, the veneer-based EWPs are stronger and more durable than solid wood of the same size. This is an outstanding advantage for constructing a building requiring high strength without a bulky appearance. Typically, LVL and PSL have about three times larger bending strength and 30% larger stiffness than the lumber products of comparable sizes [41].

Interest in veneer-based EWPs products will continue to grow for ecological reasons. For example, restrictions have been introduced in many countries on deforestation of large-diameter old-growth trees. Due to the needs in the construction market, alternative materials must be further developed. The rapid advancement in technology, along with the available raw materials, i.e., small-size fast-growth trees, would inevitably accelerate the development of EWPs [2]. Also, in recent years, the minimization of carbon footprints in construction has reached a consensus. Many architects and engineers have been designing and constructing buildings with 100% solid wood and EWPs. Meanwhile, research on the standardization of the veneerbased EWPs and expansion of their uses is no doubt required. Modernization of existing equipment and improvement of the gluing systems will allow the creation of innovative designs and special shapes that are currently not available for wood products. This will certainly expand the matrix of applications for veneer-based EWPs, as well as making them become more competitive in the market of building materials.

## **Acknowledgements**

This piece of work was financially supported by the New Brunswick Innovation Research Chair Initiative Program by the New Brunswick Innovation Foundation (Canada) and the Collaborative Research and Development Grants by Natural Sciences and Engineering Research Council of Canada (CRDPJ 523922-18).

## **Conflict of interest**

The authors declare no conflict of interest.

*Veneer-Based Engineered Wood Products in Construction DOI: http://dx.doi.org/10.5772/intechopen.102034*

## **Author details**

Elena Vladimirova\* and Meng Gong University of New Brunswick, Fredericton, Canada

\*Address all correspondence to: evladimi@unb.ca

© 2022 The Author(s). Licensee IntechOpen. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/ by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

## **References**

[1] Thelandersson S, Larsen HJ. Timber Engineering. New York, USA: Wiley; 2003

[2] Bodig J, Jayne BA. Mechanics of Wood and Wood Composites. Reprint edition. Malabar, FL: Krieger Pub Co; 1993

[3] Forest Products Laboratory (FPL). WoWood Handbook-Wood as an Engineering Material. General Technical Report FPL-GTR-190. Madison, WI: U.S. Department of Agriculture, Forest Service, Forest Products Laboratory; 2010

[4] Gong M. Lumber-Based Mass Timber Products in Construction. London, UK: IntechOpen; 2019. pp. 7-16. DOI: 10.5772/intechopen.85808

[5] Wooden Plywood Board. IndiamartCom 2021. https://www. indiamart.com/proddetail/woodenplywood-board-14009756373.html [Accessed: June 16, 2021]

[6] ThinkWood CEU. Design and Construction of Taller Wood Buildings. 2021. https://www.thinkwood.com/ wp-content/uploads/2019/09/ ThinkWood-CEU-Design-and-Construction-of-Taller-Wood-Buildings. pdf [Accessed: June 3, 2021]

[7] Vogt F, Nauth M. Carpentry. Toronto, Canada: Nelson Education Limited; 2015

[8] Ansell MP. Wood Composites. Cambridge, United Kingdom: Elsevier Science & Technology; 2015

[9] Porteous J, Kermani A. Structural Timber Design to Eurocode 5. Hoboken, United Kingdom: John Wiley & Sons, Incorporated; 2013

[10] Canada NR. Plywood 2014. https:// www.nrcan.gc.ca/our-naturalresources/forests-forestry/forestindustry-trade/forest-productsapplications/taxonomy-wood-products/ plywood/15855 [Accessed: March 24, 2021]

[11] Sellers T. Plywood and Adhesive Technology. Forest Products Utilization Laboratory, Mississippi State University, Mississippi, USA: CRC Press; 1985

[12] Filippovich A. Plywood history. From ancient Egypt to mid-twentieth century, part 1. Saint-Petersburg, Russia: Lesprominform. 2018;**3**:104-113

[13] Smulski S, editor. Engineered Wood Products: A Guide for Specifiers, Designers & Users. Madison, WI: Pfs Research Foundation; 1997

[14] Plywood - Sizes - Grades. The Canadian Wood Council - CWC 2021. https://cwc.ca/how-to-build-withwood/wood-products/panel-products/ plywood/. [Accessed: March 24, 2021]

[15] McIntyre RB. Design Features of the Mosquito. Aircraft Engineering and Aerospace Technology Emerald Insight, United Kingdom. 1944;**16**:64-67. DOI: 10.1108/eb031101

[16] Bowyer JL, Shmulsky R, Haygreen JG. Forest Products and Wood Science: An Introduction. 5th Ed. Oxford, UK: Wiley-Blackwell; 2007

[17] FAO. Yearbook of Forest Products 2000,2005,2010,2015,2019. Rome, Italy: FAO; 2021. DOI: 10.4060/cb3795m

[18] Canadian Wood Council. Wood Reference Handbook. Ottawa, Ontario, Canada: Canadian Wood Council; 1997

[19] Plywood. Wikipedia 2021. https:// en.wikipedia.org/w/index.php?title=Ply wood&oldid=1028259276 [Accessed: June 17, 2021]

[20] APA – The Engineered Wood Association. 2021. https://www. apawood.org/ [Accessed: April 14, 2021] *Veneer-Based Engineered Wood Products in Construction DOI: http://dx.doi.org/10.5772/intechopen.102034*

[21] certiWood™ Canply plywood. Plywood Design Fundamentals Canadian Plywood Association 2021. https://tolko.com/wp-content/ uploads/2020/05/Plywood-Design-Fundamentals-Canadian-Plywood-Association.pdf [Accessed: May 18, 2021]

[22] CSA Group. CSA 086:19 Engineering Design in Wood. National Standard of Canada. Toronto, Canada: CSA Group; 2021

[23] CSA Group. CAN/CSA-O80 SERIES-15 (R2020) Wood Preservation. National Standard of Canada. Toronto, Canada: CSA Group; 2020

[24] ASTM International. D5516-18 Standard Test Method for Evaluating the Flexural Properties of Fire-Retardant Treated Softwood Plywood Exposed to Elevated Temperatures. West Conshohocken, PA: ASTM International; 2018. DOI: 10.1520/D5516-18

[25] Wood Design Manual 2017. Ottawa, Ontario, Canada: Canadian Wood Council Webstore; 2017

[26] APA. Design Capacities of APA Performance-Rated Structural-Use Panels Technical Note N375. Tacoma, Washington, USA: APA The Engineered Wood Association; 1995

[27] Wood Engineering Handbook. Second ed. Englewood Cliffs, NJ: Forest Products Laboratory; Prentice Hall; 1990 http://www.matweb.com/search/ datasheet\_print.aspx?matguid=bd6620 450973496ea2578c283e9fb807 [Accessed: May 31, 2021]

[28] ASTM International. D3500-20 Standard Test Methods for Wood Structural Panels in Tension. West Conshohocken, PA: ASTM International; 2020. DOI: 10.1520/D3500-20

[29] ASTM International. D3043-17 Standard Test Methods for Structural Panels in Flexure. West Conshohocken, PA: ASTM International; 2017. DOI: 10.1520/D3043-17

[30] ASTM International. D3501-05a (2018) Standard Test Methods for Wood-Based Structural Panels in Compression. West Conshohocken, PA: ASTM International; 2018. DOI: 10.1520/ D3501-05AR18

[31] ASTM International. D2718-18 Standard Test Method for Structural Panels in Planar Shear (Rolling Shear). West Conshohocken, PA: ASTM International; 2018. DOI: 10.1520/ D2718-18

[32] ASTM International. D2719-19 Standard Test Methods for Structural Panels in Shear through-the-Thickness. West Conshohocken, PA: ASTM International; 2019. DOI: 10.1520/ D2719-19

[33] BBC Research. MFG058A Plywood Manufacturing: Global Markets to 2022. Wellesley, Massachusetts, USA: BCC Publishing; 2018

[34] Georgia-Pacific Building Products. Plytanium Sturd-I-Floor Plywood Subfloor Panels. Atlanta, Georgia, USA: Georgia-Pacific Building Products; 2021. https://buildgp.com/product/ plytanium-sturd-i-floor/ [Accessed: May 22, 2021]

[35] Georgia-Pacific Building Products. Plywood Roof Sheathing, OSB Roofing Boards. Atlanta, Georgia, USA: Georgia-Pacific Building Products; 2021. https:// buildgp.com/wood/roof-sheathing/ [Accessed: May 22, 2021]

[36] American Wood Council. Visual Guide to Floor, Roof, and Wall Systems. Washington, DC, USA: American Wood Council; 2021

[37] Laminate Veneer Lumber. The Canadian Wood Council - CWC 2021. https://cwc.ca/how-to-build-with-wood/ wood-products/structural-composite/ laminate-veneer-lumber/ [Accessed: April 14, 2021]

[38] Hsu WE. Structural Composite Lumber Manufacturing. Scotts Valley, California, USA: CreateSpace Independent Publishing Platform; 2016

[39] Gong M. Wood Technology, Lecture on Wood Products. Fredericton, Canada: University of New Brunswick; 2021

[40] Natural Resources Canada. Laminated veneer lumber. Ottawa, ON, Canada: Natural Resources Canada; 2014. https://www.nrcan.gc.ca/ournatural-resources/forests-forestry/ forest-industry-trade/forest-productsapplications/taxonomy-wood-products/ laminated-veneer-lumber/15795 [Accessed: April 14, 2021]

[41] Introduction to Wood Design 2018. Canadian Wood Council; 2018

[42] Structural Grading. WoodSolutions; 2021 https://www.woodsolutions.com. au/articles/structural-grading [Accessed: April 14, 2021]

[43] Stora Enso Wood Products GmbH. LVL by Stora Enso Technical brochure. Helsinki. Finland: Stora Enso; 2021. https://www.storaenso.com/-/media/ documents/download-center/ documents/product-brochures/woodproducts/lvl-by-stora-enso-technicalbrochure-en.pdf [Accessed: June 4, 2021]

[44] Laminated Veneer Lumber | Engineered Wood | StructureCraft. StructureCraft Builders. 2021. https:// structurecraft.com/materials/ engineered-wood/laminated-veneerlumber [Accessed: May 21, 2021]

[45] Moretti PM, Divone LV. Modern windmills. Scientific American. 1986;**254**:110-119

[46] Decker KD. Reorienting the economy to the rhythms of nature: Learning to live with intermittent energy supply. American Journal of Economics and Sociology. 2020;**79**:877- 905. DOI: 10.1111/ajes.12333

[47] Extreme Measures: At 107 Meters, The World's Largest Wind Turbine Blade Is Longer Than A Football Field. Here's What It Looks Like | GE News. 2019. https://www.ge.com/news/reports/ extreme-measures-107-meters-worldslargest-wind-turbine-blade-longerfootball-field-heres-looks-like [Accessed: May 30, 2021]

[48] Weyerhaeuser Uses Strong Scraps. Wood Business. 2014. https://www. woodbusiness.ca/weyerhaeuser-strongscraps-1859/ [Accessed: April 24, 2021]

[49] Parallel Strand Lumber. The Canadian Wood Council – CWC. 2021. https://cwc.ca/how-to-build-withwood/wood-products/structuralcomposite/parallel-strand-lumber/ [Accessed: April 16, 2021]

[50] Waste not Cambodia: Image. 2021. https://wastenotcambodia.files. wordpress.com/2012/05/parallam1.jpg [Accessed: June 16, 2021]

[51] Canada NR. Oriented Strand Lumber. 2014. https://www.nrcan.gc.ca/ our-natural-resources/forests-forestry/ forest-industry-trade/forest-productsapplications/taxonomy-wood-products/ oriented-strand-lumber/15827 [Accessed: April 24, 2021]

[52] Gould-Design-Inc. Parallel-strandlumber. Gould Design, Inc. 2013. https://goulddesigninc.com/2013/11/14/ the-abcs-of-ewp-engineered-woodproducts/parallel-strand-lumber/ [Accessed: June 16, 2021]

[53] How can I be sure that I have genuine Parallam® Plus PSL? Trus Joist Technical Support. 2021. https://www. techsupport.weyerhaeuser.com/hc/

*Veneer-Based Engineered Wood Products in Construction DOI: http://dx.doi.org/10.5772/intechopen.102034*

en-us/articles/205173710-How-can-Ibe-sure-that-I-have-genuine-Parallam-Plus-PSL [Accessed: May 30, 2021]

[54] Parallam® PSL Deep Beam Specifier's Guide. 2015

[55] Parallel Strand Lumber. Engineered Wood. StructureCraft. StructureCraft Builders. 2021. https://structurecraft. com/materials/engineered-wood/ parallel-strand-lumber [Accessed: May 21, 2021]

## **Chapter 4**
